1 | Davis Besse Reactor Pressure Vessel Head Degradation
Davis-Besse Reactor Pressure Vessel Head DegradationOverview, Lessons Learned, andNRC Actions Based on Lessons Learned
2 | Davis-Besse Reactor Pressure Vessel Head Degradation
Davis-Besse Reactor Pressure Vessel Head Degradation: Overview
BackgroundThe reactor pressure vessel (RPV) heads of pressurized water reac-tors (PWR) have penetrations for control rod drive mechanisms and instrumentation systems made from nickel-based alloys (e.g., Alloy 600) and related weld metals (Figure 1). Primary coolant and the operating conditions of PWR plants can cause cracking of these nickel-based alloys and weldments through a process called pri-mary water stress corrosion cracking (PWSCC). In response to the detection of PWSCC at several plants, the NRC issued NRC Bul-letin 2001-01, Circumferential Cracking of Reactor Pressure Vessel Head Penetration Nozzles, which requested information related to licensees programs for inspection of vessel head penetration (VHP) nozzles.
Through-Wall Cracking DetectedOn February 16, 2002, in response to Bulletin 2001-01, the Davis-Besse Nuclear Power Station (DBNPS), located in Oak Harbor, Ohio, began a refueling outage with the intent to perform work that included remotely inspecting the VHP nozzles from underneath the head focusing on the control rod drive mechanisms (CRDM). The licensee found that three CRDM nozzles had indications of through-wall axial cracking. Specifically, the licensee found these indications in CRDM nozzles 1, 2, and 3, which are located near the top of the RPV head.
Repair AttemptsThe repair of these nozzles was performed remotely from under-neath the head. On March 6, 2002, the licensee terminated the repair process on CRDM nozzle 3 to determine the cause of unusual equipment operation, and removed the machining apparatus from the nozzle. During the removal, the nozzle tipped in the downhill direction until it rested against an adjacent CRDM. If structurally sound, the surrounding steel should have held the nozzle in place.
Davis-Besse Reactor Pressure Vessel Head Degradation | 3
Figure 1b. Detail of vessel head penetration nozzles
Figure 1a. Typical pressurized water reactor
4 | Davis-Besse Reactor Pressure Vessel Head Degradation
InvestigationThe licensee investigated the condition of the RPV head surround-ing CRDM nozzle 3. The investigation included removing the CRDM nozzle and removing boric acid deposits from the top of the RPV head. Upon completing the boric acid removal on March 7, 2002, the licensee conducted a visual examination of the area and identified a large cavity in the RPV head on the downhill side of CRDM nozzle 3 (Figure 2). The corrosion was caused by borated water that leaked from the reactor coolant system onto the vessel head (Figures 3 and 4) through cracks in the nozzle and the weld that attached nozzle 3 to the RPV head (Figures 5 and 6). The remaining thickness of the RPV head in the wastage area was found to be approximately 3/8 inch. This thickness consisted of the thickness of the stainless steel cladding on the inside surface of the RPV head, which is nominally 3/8 inch thick. The stainless steel cladding is resistant to corrosion by boric acid, but it is not intended to provide structural integrity to the ves-sel. Failure of the stainless steel cladding would have resulted in a loss-of-coolant accident (LOCA). The LOCA would have resulted in actuation of the plants emergency systems.
NRC ActionsNRC issued a confirmatory action letter that required the plant to remain shut down until the situation could be satisfactorily ad-dressed and invoked the process outlined in Inspection Manual Chapter 0350, Oversight of Reactor Facilities in a Shutdown Condi-tion Due to Significant Performance and/or Operation Concern. This process establishes guidelines for the oversight of licensee per-formance during the shutdown. The process requires that specific criteria must be met before the plant can restart, to ensure that the plant is operated in a manner that provides adequate protection of public health and safety.
Davis-Besse Reactor Pressure Vessel Head Degradation | 5
Figure 2. Region of the vessel head depicted by the model and photo of the cavity after it was removed from the vessel head
6 | Davis-Besse Reactor Pressure Vessel Head Degradation
Davis-Besse Reactor Pressure Vessel Head Degradation: Lessons Learned
Operational ExperienceDuring the early 1990s, the NRC and industry recognized the potential for boric acid corrosion of an RPV head. In 1993, the industry and NRC specifically addressed the possibility of extensive RPV head wastage stemming from undetected VHP nozzle leaks involving axial cracking caused by PWSCC. The industry concluded and the NRC agreed that the likelihood of this happening was low because VHP nozzle leaks would be detected before significant RPV head degradation could occur. Nevertheless, in spite of this aware-ness and contrary to this conclusion, the DBNPS event occurred.
Lessons Learned Task ForceThe NRCs Executive Director for Operations (EDO) directed the formation of an NRC task force in response to the issues associ-ated with the DBNPS event. The objective of this task force was to independently evaluate the NRCs regulatory processes related to as-suring RPV head integrity in order to identify and recommend areas for improvement that may be applicable to either the NRC or the nuclear industry. Consistent with its charter, the task force reviewed five general areas, including: (1) reactor oversight process issues; (2) regulatory process issues; (3) research activities; (4) international practices; and (5) the NRCs Generic Issues Program.
Task Force ConclusionsThe lessons learned task force (LLTF) concluded that the DBNPS VHP nozzle leakage and RPV head degradation event was preventable. While this review was primarily introspective, this question could not be answered without considering industry activities and DBNPSs per-formance. At DBNPS, early indications of RPV corrosion were missed such as radiation element system filters being clogged by boric acid and corrosion fines, the build up of boric acid deposits on containment air cooler fins and large amounts of boric acid deposits on the RPV head. The task force concluded that the event was not prevented because: (1) the NRC, DBNPS, and the nuclear industry failed to adequately review, assess, and follow-up on relevant operating experience, (2) DBNPS
Davis-Besse Reactor Pressure Vessel Head Degradation | 7
Figure 3a. RPV head flange area showing significant amounts of boric acid deposits (photo taken during the 2000 refueling outage at DBNPS)
Figure 3b. Boric acid deposits accumulating near a CRDM nozzle (still photo of video taken during the 2000 refueling outage at DBNPS)
Figure 4a. Close-up view of the cavity
Figure 4b. Oblique view of the cavity partially showing the J-groove weld at the bottom of the cavity
8 | Davis-Besse Reactor Pressure Vessel Head Degradation
failed to assure that plant safety issues received appropriate attention, and (3) the NRC failed to integrate known or available information into its assessments of DBNPSs safety performance. Furthermore, an NRC investigation concluded that DBNPS did not adequately execute the boric acid corrosion control program in response to an NRC Generic Communication, and the NRC did not adequately review the industry implementation of long term commitments, such as the commitment to maintain a boric acid corrosion control program.
NRC ActionsAs a result of its review, the task force determined that the NRC should take specific actions to address contributing factors that led to the DB-NPS event. The recommendations made involved the following areas: 1) stress corrosion cracking, 2) reactor coolant pressure boundary integrity, 3) operational experience and 4) inspection and program management. Select examples of NRC actions taken to address recommendations of the LLTF in these areas are described in a later section.
Davis-Besse Reactor Pressure Vessel Head Degradation: NRC Actions Based on Lessons Learned
The LLTF developed recommendations in key technical and pro-grammatic areas. Examples of some of the actions taken by the NRC to address the recommendations of the task force in the areas of stress corrosion cracking, operating experience, and inspection and program management are discussed below.
Stress Corrosion CrackingNRC Order EA-03-009 was issued requiring all licensees with plants susceptible to RPV head degradation to visually inspect the reac-tor vessel head surface area for indications of leakage and boric acid accumulation, as well as inspect head penetrations using methods to detect cracks before leakage starts.
The NRC worked with the American Society of Mechanical Engineers (ASME) to develop Code Case N-729-1 to develop long-term inspection
Davis-Besse Reactor Pressure Vessel Head Degradation | 9
Figure 6. Top photo: Top view of the J-groove weld with an arrow pointing to a crack Top-right photo: Polished cross section of the area shown in the top photo showing the through-wall crack in the J-groove weld
Top View of J-Groove Weld
Figure 5. Schematic of the nozzle penetration cross section showing the leak path of the reactor coolant
10 | Davis-Besse Reactor Pressure Vessel Head Degradation
requirements of RPV heads into the ASME Code. The finalized inspec-tion requirements will be incorporated into 10 CFR 50.55a and allow the rescission of NRC Order EA-